DOI: 10.17188/1475754
title: Materials Data on Sr2Ca2TiMn3O10 by Materials Project

description: Sr2Ca2TiMn3O10 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are sixteen inequivalent Sr2+ sites. In the first Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–2.83 Å. In the second Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.43–3.14 Å. In the third Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.52–3.05 Å. In the fourth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–2.80 Å. In the fifth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.36–3.05 Å. In the sixth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–3.11 Å. In the seventh Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–3.05 Å. In the eighth Sr2+ site, Sr2+ is bonded in a 2-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.35–2.95 Å. In the ninth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.43–3.11 Å. In the tenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.51–3.04 Å. In the eleventh Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–3.05 Å. In the twelfth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–2.84 Å. In the thirteenth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–2.81 Å. In the fourteenth Sr2+ site, Sr2+ is bonded in a 2-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.38–2.92 Å. In the fifteenth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–2.81 Å. In the sixteenth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.37–2.85 Å. There are sixteen inequivalent Ca2+ sites. In the first Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.24–2.64 Å. In the second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.89 Å. In the third Ca2+ site, Ca2+ is bonded in a 2-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.28–3.07 Å. In the fourth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.24–2.98 Å. In the fifth Ca2+ site, Ca2+ is bonded in a 2-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–3.01 Å. In the sixth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.39–2.92 Å. In the seventh Ca2+ site, Ca2+ is bonded in a 2-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.25–2.97 Å. In the eighth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.26–2.87 Å. In the ninth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.24–2.98 Å. In the tenth Ca2+ site, Ca2+ is bonded in a 5-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.29–2.76 Å. In the eleventh Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.23–2.67 Å. In the twelfth Ca2+ site, Ca2+ is bonded in a 2-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.26–3.06 Å. In the thirteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.41–2.93 Å. In the fourteenth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.24–2.76 Å. In the fifteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.41–3.00 Å. In the sixteenth Ca2+ site, Ca2+ is bonded in a 5-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.27–2.80 Å. There are eight inequivalent Ti4+ sites. In the first Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share a cornercorner with one MnO6 octahedra, corners with three TiO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–15°. There are a spread of Ti–O bond distances ranging from 1.90–2.12 Å. In the second Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share a cornercorner with one MnO6 octahedra, corners with three TiO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–17°. There are a spread of Ti–O bond distances ranging from 1.90–2.15 Å. In the third Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share a cornercorner with one MnO6 octahedra, corners with three TiO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 8–14°. There are a spread of Ti–O bond distances ranging from 1.87–2.09 Å. In the fourth Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–11°. There are a spread of Ti–O bond distances ranging from 1.95–2.03 Å. In the fifth Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share a cornercorner with one MnO6 octahedra, corners with three TiO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 13–16°. There are a spread of Ti–O bond distances ranging from 1.87–2.07 Å. In the sixth Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share corners with four TiO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 14–17°. There are a spread of Ti–O bond distances ranging from 1.90–2.06 Å. In the seventh Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share corners with four TiO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–16°. There are a spread of Ti–O bond distances ranging from 1.89–2.09 Å. In the eighth Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share corners with four TiO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 13–16°. There are a spread of Ti–O bond distances ranging from 1.91–2.04 Å. There are twenty-four inequivalent Mn+2.67+ sites. In the first Mn+2.67+ site, Mn+2.67+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 3–8°. There are a spread of Mn–O bond distances ranging from 1.96–2.11 Å. In the second Mn+2.67+ site, Mn+2.67+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 5–12°. There are a spread of Mn–O bond distances ranging from 2.02–2.14 Å. In the third Mn+2.67+ site, Mn+2.67+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 4–10°. There are a spread of Mn–O bond distances ranging from 1.98–2.11 Å. In the fourth Mn+2.67+ site, Mn+2.67+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four TiO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–14°. There are a spread of Mn–O bond distances ranging from 2.09–2.16 Å. In the fifth Mn+2.67+ site, Mn+2.67+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one TiO6 octahedra, corners with three MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 4–11°. There are a spread of Mn–O bond distances ranging from 1.95–2.16 Å. In the sixth Mn+2.67+ site, Mn+2.67+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one TiO6 octahedra, corners with three MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 8–12°. There are a spread of Mn–O bond distances ranging from 1.95–2.04 Å. In the seventh Mn+2.67+ site, Mn+2.67+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one TiO6 octahedra, corners with three MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 3–7°. There are a spread of Mn–O bond distances ranging from 1.96–2.24 Å. In the eighth Mn+2.67+ site, Mn+2.67+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one TiO6 octahedra, corners with three MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–10°. There are a spread of Mn–O bond distances ranging from 1.92–2.05 Å. In the ninth Mn+2.67+ site, Mn+2.67+ is bonded to four O2- atoms to form MnO4 tetrahedra that share a cornercorner with one TiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 23–31°. There are a spread of Mn–O bond distances ranging from 1.89–1.98 Å. In the tenth Mn+2.67+ site, Mn+2.67+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 22–27°. There are a spread of Mn–O bond distances ranging from 1.91–2.00 Å. In the eleventh Mn+2.67+ site, Mn+2.67+ is bonded to four O2- atoms to form MnO4 tetrahedra that share a cornercorner with one TiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–38°. There are a spread of Mn–O bond distances ranging from 2.02–2.09 Å. In the twelfth Mn+2.67+ site, Mn+2.67+ is bonded to four O2- atoms to form MnO4 tetrahedra that share a cornercorner with one TiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 20–33°. There are a spread of Mn–O bond distances ranging from 1.97–2.08 Å. In the thirteenth Mn+2.67+ site, Mn+2.67+ is bonded to four O2- atoms to form MnO4 tetrahedra that share a cornercorner with one TiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 18–36°. There are a spread of Mn–O bond distances ranging from 1.88–2.00 Å. In the fourteenth Mn+